#------------------------------------------------------------------------------
#$Date: 2016-03-22 23:16:05 +0200 (Tue, 22 Mar 2016) $
#$Revision: 179053 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/15/4301550.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4301550
loop_
_publ_author_name
'Chun-Hong Li'
'Kun-Lin Huang'
'Ying-Nan Chi'
'Xi Liu'
'Zhan-Gang Han'
'Long Shen'
'Chang-Wen Hu'
_publ_section_title
;
Lanthanide-Organic Cation Frameworks with Zeolite Gismondine Topology and
Large Cavities from Intersected Channels Templated by Polyoxometalate
Counterions
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2010
_journal_page_last               2017
_journal_paper_doi               10.1021/ic801846h
_journal_volume                  48
_journal_year                    2009
_chemical_formula_sum            'C28 H48 Ce4 Mo12 N4 O74 Si'
_chemical_formula_weight         3364.55
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 133.1180(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   30.753(3)
_cell_length_b                   15.7285(13)
_cell_length_c                   22.119(2)
_cell_measurement_reflns_used    6271
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.258
_cell_measurement_theta_min      2.395
_cell_volume                     7809.7(12)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0309
_diffrn_reflns_av_sigmaI/netI    0.1728
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -36
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            19414
_diffrn_reflns_theta_full        25.01
_diffrn_reflns_theta_max         25.01
_diffrn_reflns_theta_min         1.58
_exptl_absorpt_coefficient_mu    4.279
_exptl_absorpt_correction_T_max  0.425
_exptl_absorpt_correction_T_min  0.288
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs(Sheldrick,1996)
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.862
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       cubic
_exptl_crystal_F_000             6344
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.20
_refine_diff_density_max         3.950
_refine_diff_density_min         -3.304
_refine_diff_density_rms         0.240
_refine_ls_extinction_coef       0.00041(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.000
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     580
_refine_ls_number_reflns         6877
_refine_ls_number_restraints     102
_refine_ls_restrained_S_all      1.023
_refine_ls_R_factor_all          0.1250
_refine_ls_R_factor_gt           0.0847
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0540P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1901
_refine_ls_wR_factor_ref         0.2072
_reflns_number_gt                4066
_reflns_number_total             6877
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic801846h_si_002_2.cif
_cod_data_source_block           2
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        7809.6(12)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               4301550
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ce1 Ce 0.39008(5) -0.13669(7) 0.82747(6) 0.0210(3) Uani 1 1 d . . .
Ce2 Ce 0.33064(5) 0.12852(6) 0.98581(6) 0.0190(3) Uani 1 1 d . . .
Mo1 Mo 0.5000 0.8605(2) 0.2500 0.0865(14) Uani 1 2 d SU . .
Mo2 Mo 0.63118(11) 0.74764(14) 0.40949(12) 0.0649(9) Uani 1 1 d . . .
Mo3 Mo 0.42354(9) 0.74761(13) 0.29145(12) 0.0390(6) Uani 1 1 d . . .
Mo4 Mo 0.55444(8) 0.63531(12) 0.45145(11) 0.0296(5) Uani 1 1 d . . .
Mo5 Mo 0.42392(10) 0.52275(13) 0.29114(14) 0.0449(6) Uani 1 1 d . . .
Mo6 Mo 0.37050(10) 0.52331(19) 0.09013(13) 0.0672(9) Uani 1 1 d . . .
Mo7 Mo 0.5000 0.40969(18) 0.2500 0.0681(12) Uani 1 2 d S . .
N1 N 0.3380(7) 0.0019(8) 0.7416(9) 0.019(3) Uani 1 1 d . . .
N2 N 0.3664(6) 0.2651(9) 0.9637(8) 0.019(3) Uani 1 1 d U . .
O1 O 0.5427(10) 0.7174(14) 0.2745(14) 0.019(6) Uani 0.50 1 d P . .
O2 O 0.4840(10) 0.6412(13) 0.3058(14) 0.018(5) Uani 0.50 1 d PU . .
O3 O 0.4603(10) 0.5495(15) 0.2274(15) 0.023(6) Uani 0.50 1 d PU . .
O4 O 0.4439(10) 0.6405(14) 0.1545(14) 0.016(5) Uani 0.50 1 d PU . .
O5 O 0.5782(10) 0.8377(13) 0.3598(13) 0.098(7) Uani 1 1 d U . .
O6 O 0.4677(10) 0.8376(13) 0.2950(13) 0.096(7) Uani 1 1 d U . .
O7 O 0.6042(7) 0.7192(10) 0.4622(11) 0.065(5) Uani 1 1 d U . .
O8 O 0.4937(6) 0.7211(9) 0.3997(10) 0.069(6) Uani 1 1 d . . .
O9 O 0.3955(6) 0.6350(9) 0.2796(10) 0.066(5) Uani 1 1 d . . .
O10 O 0.4944(7) 0.5519(9) 0.4018(10) 0.067(6) Uani 1 1 d . . .
O11 O 0.3660(8) 0.5154(12) 0.1721(11) 0.077(6) Uani 1 1 d U . .
O12 O 0.4286(9) 0.4311(14) 0.1470(13) 0.097(7) Uani 1 1 d U . .
O13 O 0.6296(8) 0.7504(11) 0.3233(11) 0.073(5) Uani 1 1 d U . .
O14 O 0.6003(8) 0.5501(11) 0.4583(12) 0.069(5) Uani 1 1 d U . .
O15 O 0.3383(8) 0.6393(10) 0.0660(11) 0.063(5) Uani 1 1 d U . .
O16 O 0.5338(8) 0.4364(11) 0.2065(10) 0.075(6) Uani 1 1 d U . .
O17 O 0.5000 0.9645(14) 0.2500 0.065(7) Uani 1 2 d S . .
O18 O 0.6906(10) 0.8040(14) 0.4841(13) 0.105(7) Uani 1 1 d U . .
O19 O 0.3888(6) 0.7998(12) 0.3135(9) 0.068(6) Uani 1 1 d . . .
O20 O 0.5786(8) 0.6356(8) 0.5444(9) 0.050(5) Uani 1 1 d . . .
O21 O 0.3864(7) 0.4702(11) 0.3063(9) 0.060(5) Uani 1 1 d . . .
O22 O 0.3088(5) 0.4696(9) 0.0139(8) 0.046(4) Uani 1 1 d . . .
O23 O 0.4806(12) 0.3057(16) 0.2229(16) 0.041(8) Uani 0.50 1 d PU . .
O24 O 0.3660(7) -0.0274(9) 0.8831(9) 0.042(4) Uani 1 1 d . . .
O25 O 0.3249(6) 0.0968(8) 0.8723(9) 0.036(4) Uani 1 1 d . . .
O26 O 0.3767(6) -0.1144(9) 0.7044(9) 0.037(4) Uani 1 1 d . . .
O27 O 0.3415(6) -0.0460(8) 0.5911(8) 0.037(4) Uani 1 1 d . . .
O28 O 0.2532(5) 0.2339(8) 0.8733(8) 0.027(3) Uani 1 1 d . . .
O29 O 0.2227(6) 0.3489(8) 0.7943(8) 0.036(4) Uani 1 1 d . . .
O30 O 0.4401(5) 0.1459(8) 1.0675(7) 0.025(3) Uani 1 1 d . . .
O31 O 0.5196(5) 0.2188(8) 1.1125(8) 0.035(4) Uani 1 1 d . . .
O32 O 0.3408(6) -0.2044(9) 0.8743(9) 0.050(4) Uani 1 1 d . . .
H32C H 0.3413 -0.2581 0.8703 0.060 Uiso 1 1 d R . .
H32A H 0.3050 -0.1883 0.8452 0.060 Uiso 1 1 d R . .
O33 O 0.4693(7) -0.1318(10) 0.9920(8) 0.058(5) Uani 1 1 d . . .
H33B H 0.4685 -0.1755 1.0138 0.070 Uiso 1 1 d R . .
H33C H 0.4669 -0.0867 1.0107 0.070 Uiso 1 1 d R . .
O34 O 0.4728(6) -0.0241(9) 0.8775(9) 0.047(4) Uani 1 1 d . . .
H34B H 0.4582 0.0162 0.8427 0.056 Uiso 1 1 d R . .
H34C H 0.5012 -0.0471 0.8848 0.056 Uiso 1 1 d R . .
O35 O 0.3660(6) -0.2804(8) 0.7618(8) 0.050(4) Uani 1 1 d . . .
H35B H 0.3287 -0.2891 0.7257 0.060 Uiso 1 1 d R . .
H35C H 0.3829 -0.3197 0.7980 0.060 Uiso 1 1 d R . .
O36 O 0.3786(7) -0.0165(8) 1.0162(9) 0.050(5) Uani 1 1 d . . .
H36B H 0.3664 -0.0412 0.9727 0.060 Uiso 1 1 d R . .
H36C H 0.3757 -0.0492 1.0439 0.060 Uiso 1 1 d R . .
O37 O 0.2470(7) 0.0285(10) 0.8872(10) 0.069(6) Uani 1 1 d . . .
H37B H 0.2212 0.0295 0.8909 0.083 Uiso 1 1 d R . .
H37C H 0.2590 -0.0221 0.8929 0.083 Uiso 1 1 d R . .
O38 O 0.2455(6) 0.1603(8) 0.9792(9) 0.044(4) Uani 1 1 d . . .
H38B H 0.2515 0.2054 1.0053 0.053 Uiso 1 1 d R . .
H38C H 0.2385 0.1189 0.9963 0.053 Uiso 1 1 d R . .
O39 O 0.3675(6) 0.2338(8) 1.1058(7) 0.032(3) Uani 1 1 d . . .
H39B H 0.3435 0.2753 1.0869 0.038 Uiso 1 1 d R . .
H39C H 0.4022 0.2527 1.1318 0.038 Uiso 1 1 d R . .
O40 O 0.7640(8) 0.1470(11) 0.1660(12) 0.079(6) Uani 1 1 d . . .
H40C H 0.8012 0.1448 0.1945 0.095 Uiso 1 1 d R . .
H40D H 0.7463 0.1601 0.1165 0.095 Uiso 1 1 d R . .
Si1 Si 0.5000 0.6347(5) 0.2500 0.0213(16) Uani 1 2 d S . .
C1 C 0.3379(8) 0.0413(11) 0.8460(10) 0.018(4) Uani 1 1 d . . .
C2 C 0.3157(8) 0.0577(11) 0.7621(11) 0.017(4) Uani 1 1 d . . .
C3 C 0.2745(9) 0.1168(11) 0.7067(11) 0.027(5) Uani 1 1 d . . .
H3 H 0.2560 0.1496 0.7188 0.032 Uiso 1 1 calc R . .
C4 C 0.2598(11) 0.1284(14) 0.6328(14) 0.049(6) Uani 1 1 d . . .
H4 H 0.2327 0.1702 0.5955 0.059 Uiso 1 1 calc R . .
C5 C 0.2863(8) 0.0763(12) 0.6155(11) 0.027(5) Uani 1 1 d . . .
H5 H 0.2785 0.0836 0.5672 0.032 Uiso 1 1 calc R . .
C6 C 0.3248(8) 0.0128(13) 0.6717(12) 0.029(5) Uani 1 1 d . . .
C7 C 0.3505(9) -0.0521(12) 0.6545(12) 0.024(5) Uani 1 1 d . . .
C8 C 0.2621(8) 0.3021(11) 0.8528(11) 0.018(4) Uani 1 1 d . . .
C9 C 0.3270(9) 0.3242(12) 0.9066(12) 0.030(5) Uani 1 1 d . . .
C10 C 0.3439(9) 0.3997(12) 0.8949(12) 0.031(5) Uani 1 1 d . . .
H10 H 0.3158 0.4394 0.8555 0.037 Uiso 1 1 calc R . .
C11 C 0.4062(9) 0.4140(13) 0.9459(12) 0.031(5) Uani 1 1 d . . .
H11 H 0.4198 0.4631 0.9398 0.038 Uiso 1 1 calc R . .
C12 C 0.4461(9) 0.3534(12) 1.0046(12) 0.030(5) Uani 1 1 d . . .
H12 H 0.4869 0.3619 1.0390 0.036 Uiso 1 1 calc R . .
C13 C 0.4253(8) 0.2808(11) 1.0117(11) 0.020(4) Uani 1 1 d U . .
C14 C 0.4643(8) 0.2104(12) 1.0683(11) 0.022(4) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O31 Ce1 O26 86.9(5) 5_657 . ?
O31 Ce1 O24 134.2(5) 5_657 . ?
O26 Ce1 O24 123.9(4) . . ?
O31 Ce1 O35 67.6(4) 5_657 . ?
O26 Ce1 O35 74.4(5) . . ?
O24 Ce1 O35 146.5(5) . . ?
O31 Ce1 O29 137.3(4) 5_657 4_546 ?
O26 Ce1 O29 76.7(5) . 4_546 ?
O24 Ce1 O29 86.3(5) . 4_546 ?
O35 Ce1 O29 70.1(4) . 4_546 ?
O31 Ce1 O32 108.7(4) 5_657 . ?
O26 Ce1 O32 142.7(5) . . ?
O24 Ce1 O32 68.5(5) . . ?
O35 Ce1 O32 80.7(5) . . ?
O29 Ce1 O32 68.9(4) 4_546 . ?
O31 Ce1 N1 137.4(4) 5_657 . ?
O26 Ce1 N1 61.5(4) . . ?
O24 Ce1 N1 62.7(4) . . ?
O35 Ce1 N1 122.8(5) . . ?
O29 Ce1 N1 65.8(4) 4_546 . ?
O32 Ce1 N1 113.7(4) . . ?
O31 Ce1 O34 73.7(4) 5_657 . ?
O26 Ce1 O34 75.8(4) . . ?
O24 Ce1 O34 81.8(4) . . ?
O35 Ce1 O34 131.6(5) . . ?
O29 Ce1 O34 136.3(4) 4_546 . ?
O32 Ce1 O34 140.4(5) . . ?
N1 Ce1 O34 71.4(4) . . ?
O31 Ce1 O33 68.8(5) 5_657 . ?
O26 Ce1 O33 143.8(5) . . ?
O24 Ce1 O33 67.0(5) . . ?
O35 Ce1 O33 116.7(5) . . ?
O29 Ce1 O33 139.2(5) 4_546 . ?
O32 Ce1 O33 72.7(5) . . ?
N1 Ce1 O33 120.4(5) . . ?
O34 Ce1 O33 71.9(5) . . ?
O25 Ce2 O27 136.6(4) . 6_556 ?
O25 Ce2 O37 70.4(5) . . ?
O27 Ce2 O37 83.5(5) 6_556 . ?
O25 Ce2 O30 83.2(4) . . ?
O27 Ce2 O30 97.3(4) 6_556 . ?
O37 Ce2 O30 140.5(5) . . ?
O25 Ce2 O36 73.2(4) . . ?
O27 Ce2 O36 66.5(4) 6_556 . ?
O37 Ce2 O36 74.3(6) . . ?
O30 Ce2 O36 70.1(4) . . ?
O25 Ce2 O28 76.5(4) . . ?
O27 Ce2 O28 133.8(4) 6_556 . ?
O37 Ce2 O28 80.7(5) . . ?
O30 Ce2 O28 121.8(4) . . ?
O36 Ce2 O28 145.7(4) . . ?
O25 Ce2 O38 128.7(5) . . ?
O27 Ce2 O38 68.5(4) 6_556 . ?
O37 Ce2 O38 70.7(5) . . ?
O30 Ce2 O38 146.0(4) . . ?
O36 Ce2 O38 125.0(4) . . ?
O28 Ce2 O38 65.3(4) . . ?
O25 Ce2 N2 73.7(4) . . ?
O27 Ce2 N2 143.5(4) 6_556 . ?
O37 Ce2 N2 132.3(5) . . ?
O30 Ce2 N2 61.1(4) . . ?
O36 Ce2 N2 123.1(4) . . ?
O28 Ce2 N2 60.9(4) . . ?
O38 Ce2 N2 111.9(4) . . ?
O25 Ce2 O39 147.3(4) . . ?
O27 Ce2 O39 72.2(4) 6_556 . ?
O37 Ce2 O39 139.0(4) . . ?
O30 Ce2 O39 76.5(4) . . ?
O36 Ce2 O39 121.6(4) . . ?
O28 Ce2 O39 92.6(4) . . ?
O38 Ce2 O39 69.8(4) . . ?
N2 Ce2 O39 74.1(4) . . ?
O17 Mo1 O6 101.2(7) . 2_655 ?
O17 Mo1 O6 101.2(7) . . ?
O6 Mo1 O6 157.7(13) 2_655 . ?
O17 Mo1 O5 100.5(6) . . ?
O6 Mo1 O5 88.6(9) 2_655 . ?
O6 Mo1 O5 87.3(9) . . ?
O17 Mo1 O5 100.5(6) . 2_655 ?
O6 Mo1 O5 87.3(9) 2_655 2_655 ?
O6 Mo1 O5 88.6(9) . 2_655 ?
O5 Mo1 O5 158.9(12) . 2_655 ?
O17 Mo1 O1 155.6(5) . 2_655 ?
O6 Mo1 O1 96.0(9) 2_655 2_655 ?
O6 Mo1 O1 62.8(8) . 2_655 ?
O5 Mo1 O1 97.1(8) . 2_655 ?
O5 Mo1 O1 62.8(8) 2_655 2_655 ?
O17 Mo1 O1 155.6(5) . . ?
O6 Mo1 O1 62.8(8) 2_655 . ?
O6 Mo1 O1 96.0(9) . . ?
O5 Mo1 O1 62.8(8) . . ?
O5 Mo1 O1 97.1(8) 2_655 . ?
O1 Mo1 O1 48.8(11) 2_655 . ?
O18 Mo2 O15 102.1(10) . 2_655 ?
O18 Mo2 O5 96.0(11) . . ?
O15 Mo2 O5 161.8(9) 2_655 . ?
O18 Mo2 O13 104.3(9) . . ?
O15 Mo2 O13 88.5(7) 2_655 . ?
O5 Mo2 O13 88.7(8) . . ?
O18 Mo2 O7 99.4(8) . . ?
O15 Mo2 O7 87.2(7) 2_655 . ?
O5 Mo2 O7 88.1(8) . . ?
O13 Mo2 O7 156.4(8) . . ?
O18 Mo2 O1 156.2(10) . . ?
O15 Mo2 O1 95.9(8) 2_655 . ?
O5 Mo2 O1 67.2(8) . . ?
O13 Mo2 O1 60.4(8) . . ?
O7 Mo2 O1 97.0(8) . . ?
O18 Mo2 O4 158.8(9) . 2_655 ?
O15 Mo2 O4 67.2(7) 2_655 2_655 ?
O5 Mo2 O4 95.0(9) . 2_655 ?
O13 Mo2 O4 94.1(8) . 2_655 ?
O7 Mo2 O4 62.9(7) . 2_655 ?
O1 Mo2 O4 44.6(8) . 2_655 ?
O19 Mo3 O13 104.4(8) . 2_655 ?
O19 Mo3 O8 98.3(8) . . ?
O13 Mo3 O8 157.3(8) 2_655 . ?
O19 Mo3 O9 100.3(9) . . ?
O13 Mo3 O9 86.6(7) 2_655 . ?
O8 Mo3 O9 89.2(6) . . ?
O19 Mo3 O6 101.6(10) . . ?
O13 Mo3 O6 88.6(8) 2_655 . ?
O8 Mo3 O6 87.0(8) . . ?
O9 Mo3 O6 158.1(9) . . ?
O19 Mo3 O1 158.2(8) . 2_655 ?
O13 Mo3 O1 60.3(8) 2_655 2_655 ?
O8 Mo3 O1 97.8(8) . 2_655 ?
O9 Mo3 O1 94.4(8) . 2_655 ?
O6 Mo3 O1 64.8(8) . 2_655 ?
O19 Mo3 O2 156.5(8) . . ?
O13 Mo3 O2 94.4(8) 2_655 . ?
O8 Mo3 O2 63.6(7) . . ?
O9 Mo3 O2 66.4(7) . . ?
O6 Mo3 O2 92.7(9) . . ?
O1 Mo3 O2 45.2(7) 2_655 . ?
O20 Mo4 O14 103.3(8) . . ?
O20 Mo4 O10 99.0(8) . . ?
O14 Mo4 O10 86.2(7) . . ?
O20 Mo4 O7 101.8(8) . . ?
O14 Mo4 O7 89.4(7) . . ?
O10 Mo4 O7 159.3(8) . . ?
O20 Mo4 O8 99.7(8) . . ?
O14 Mo4 O8 157.0(8) . . ?
O10 Mo4 O8 88.6(6) . . ?
O7 Mo4 O8 87.6(7) . . ?
O20 Mo4 O2 156.9(8) . . ?
O14 Mo4 O2 94.4(8) . . ?
O10 Mo4 O2 67.2(7) . . ?
O7 Mo4 O2 93.0(8) . . ?
O8 Mo4 O2 63.0(8) . . ?
O20 Mo4 O4 159.7(8) . 2_655 ?
O14 Mo4 O4 65.3(7) . 2_655 ?
O10 Mo4 O4 97.0(8) . 2_655 ?
O7 Mo4 O4 62.9(8) . 2_655 ?
O8 Mo4 O4 93.2(8) . 2_655 ?
O2 Mo4 O4 43.1(7) . 2_655 ?
O21 Mo5 O16 101.8(9) . 2_655 ?
O21 Mo5 O9 100.0(8) . . ?
O16 Mo5 O9 158.2(8) 2_655 . ?
O21 Mo5 O10 101.6(8) . . ?
O16 Mo5 O10 88.9(7) 2_655 . ?
O9 Mo5 O10 87.9(6) . . ?
O21 Mo5 O11 97.3(8) . . ?
O16 Mo5 O11 88.3(7) 2_655 . ?
O9 Mo5 O11 87.8(7) . . ?
O10 Mo5 O11 161.1(8) . . ?
O21 Mo5 O3 154.7(8) . . ?
O16 Mo5 O3 62.5(8) 2_655 . ?
O9 Mo5 O3 96.6(8) . . ?
O10 Mo5 O3 97.9(8) . . ?
O11 Mo5 O3 64.4(8) . . ?
O21 Mo5 O2 157.2(8) . . ?
O16 Mo5 O2 95.8(8) 2_655 . ?
O9 Mo5 O2 63.6(7) . . ?
O10 Mo5 O2 64.0(8) . . ?
O11 Mo5 O2 97.7(8) . . ?
O3 Mo5 O2 48.0(8) . . ?
O22 Mo6 O14 101.3(8) . 2_655 ?
O22 Mo6 O11 99.0(8) . . ?
O14 Mo6 O11 159.7(8) 2_655 . ?
O22 Mo6 O12 100.6(8) . . ?
O14 Mo6 O12 87.1(8) 2_655 . ?
O11 Mo6 O12 88.2(8) . . ?
O22 Mo6 O15 100.4(7) . . ?
O14 Mo6 O15 89.2(7) 2_655 . ?
O11 Mo6 O15 88.2(7) . . ?
O12 Mo6 O15 159.0(8) . . ?
O22 Mo6 O3 155.8(7) . . ?
O14 Mo6 O3 95.8(8) 2_655 . ?
O11 Mo6 O3 64.6(8) . . ?
O12 Mo6 O3 63.2(8) . . ?
O15 Mo6 O3 96.7(8) . . ?
O22 Mo6 O4 156.7(7) . . ?
O14 Mo6 O4 63.4(7) 2_655 . ?
O11 Mo6 O4 97.5(8) . . ?
O12 Mo6 O4 96.3(8) . . ?
O15 Mo6 O4 63.8(7) . . ?
O3 Mo6 O4 47.5(8) . . ?
O23 Mo7 O23 32.4(16) 2_655 . ?
O23 Mo7 O12 84.5(11) 2_655 2_655 ?
O23 Mo7 O12 116.9(11) . 2_655 ?
O23 Mo7 O12 116.9(11) 2_655 . ?
O23 Mo7 O12 84.5(11) . . ?
O12 Mo7 O12 158.6(14) 2_655 . ?
O23 Mo7 O16 102.5(13) 2_655 2_655 ?
O23 Mo7 O16 102.3(12) . 2_655 ?
O12 Mo7 O16 86.2(8) 2_655 2_655 ?
O12 Mo7 O16 89.1(7) . 2_655 ?
O23 Mo7 O16 102.3(12) 2_655 . ?
O23 Mo7 O16 102.5(12) . . ?
O12 Mo7 O16 89.1(7) 2_655 . ?
O12 Mo7 O16 86.2(8) . . ?
O16 Mo7 O16 154.2(12) 2_655 . ?
O23 Mo7 O3 143.3(11) 2_655 2_655 ?
O23 Mo7 O3 163.8(12) . 2_655 ?
O12 Mo7 O3 63.9(9) 2_655 2_655 ?
O12 Mo7 O3 95.7(9) . 2_655 ?
O16 Mo7 O3 94.0(8) 2_655 2_655 ?
O16 Mo7 O3 61.4(8) . 2_655 ?
O23 Mo7 O3 163.8(12) 2_655 . ?
O23 Mo7 O3 143.3(11) . . ?
O12 Mo7 O3 95.7(9) 2_655 . ?
O12 Mo7 O3 63.9(9) . . ?
O16 Mo7 O3 61.4(8) 2_655 . ?
O16 Mo7 O3 94.0(8) . . ?
O3 Mo7 O3 46.9(11) 2_655 . ?
C6 N1 C2 119.0(16) . . ?
C6 N1 Ce1 120.6(12) . . ?
C2 N1 Ce1 119.6(11) . . ?
C9 N2 C13 118.0(16) . . ?
C9 N2 Ce2 121.2(12) . . ?
C13 N2 Ce2 120.8(11) . . ?
Si1 O1 O4 54.0(10) . 2_655 ?
Si1 O1 O2 55.4(10) . 2_655 ?
O4 O1 O2 95.2(14) 2_655 2_655 ?
Si1 O1 Mo2 123.3(12) . . ?
O4 O1 Mo2 69.3(10) 2_655 . ?
O2 O1 Mo2 137.8(13) 2_655 . ?
Si1 O1 Mo3 123.1(11) . 2_655 ?
O4 O1 Mo3 138.3(13) 2_655 2_655 ?
O2 O1 Mo3 67.7(10) 2_655 2_655 ?
Mo2 O1 Mo3 97.5(9) . 2_655 ?
Si1 O1 Mo1 117.4(11) . . ?
O4 O1 Mo1 125.2(12) 2_655 . ?
O2 O1 Mo1 124.9(13) 2_655 . ?
Mo2 O1 Mo1 94.3(7) . . ?
Mo3 O1 Mo1 94.2(8) 2_655 . ?
Si1 O2 O4 55.6(10) . 2_655 ?
Si1 O2 O1 57.5(10) . 2_655 ?
O4 O2 O1 93.8(15) 2_655 2_655 ?
Si1 O2 Mo4 124.5(12) . . ?
O4 O2 Mo4 69.2(11) 2_655 . ?
O1 O2 Mo4 138.2(13) 2_655 . ?
Si1 O2 Mo3 124.6(12) . . ?
O4 O2 Mo3 133.5(13) 2_655 . ?
O1 O2 Mo3 67.1(10) 2_655 . ?
Mo4 O2 Mo3 96.6(8) . . ?
Si1 O2 Mo5 116.2(11) . . ?
O4 O2 Mo5 129.7(13) 2_655 . ?
O1 O2 Mo5 124.9(13) 2_655 . ?
Mo4 O2 Mo5 93.2(7) . . ?
Mo3 O2 Mo5 93.9(8) . . ?
Si1 O3 Mo6 120.4(12) . . ?
Si1 O3 Mo5 121.4(12) . . ?
Mo6 O3 Mo5 97.0(8) . . ?
Si1 O3 Mo7 121.2(12) . . ?
Mo6 O3 Mo7 95.2(8) . . ?
Mo5 O3 Mo7 95.4(8) . . ?
Si1 O4 O2 58.1(10) . 2_655 ?
Si1 O4 O1 58.5(10) . 2_655 ?
O2 O4 O1 95.8(15) 2_655 2_655 ?
Si1 O4 Mo4 125.3(11) . 2_655 ?
O2 O4 Mo4 67.6(10) 2_655 2_655 ?
O1 O4 Mo4 137.6(13) 2_655 2_655 ?
Si1 O4 Mo2 124.5(12) . 2_655 ?
O2 O4 Mo2 132.5(13) 2_655 2_655 ?
O1 O4 Mo2 66.0(10) 2_655 2_655 ?
Mo4 O4 Mo2 95.9(8) 2_655 2_655 ?
Si1 O4 Mo6 117.6(11) . . ?
O2 O4 Mo6 129.9(13) 2_655 . ?
O1 O4 Mo6 125.5(12) 2_655 . ?
Mo4 O4 Mo6 91.9(8) 2_655 . ?
Mo2 O4 Mo6 93.0(7) 2_655 . ?
Mo2 O5 Mo1 135.5(11) . . ?
Mo1 O6 Mo3 137.7(12) . . ?
Mo2 O7 Mo4 137.7(11) . . ?
Mo3 O8 Mo4 136.1(10) . . ?
Mo3 O9 Mo5 135.9(9) . . ?
Mo4 O10 Mo5 135.6(10) . . ?
Mo6 O11 Mo5 133.8(10) . . ?
Mo7 O12 Mo6 137.5(11) . . ?
Mo3 O13 Mo2 141.0(11) 2_655 . ?
Mo6 O14 Mo4 138.5(10) 2_655 . ?
Mo2 O15 Mo6 135.9(9) 2_655 . ?
Mo5 O16 Mo7 140.3(11) 2_655 . ?
O23 O23 Mo7 73.8(8) 2_655 . ?
C1 O24 Ce1 124.5(11) . . ?
C1 O25 Ce2 142.6(12) . . ?
C7 O26 Ce1 126.3(12) . . ?
C7 O27 Ce2 143.9(12) . 6 ?
C8 O28 Ce2 127.9(11) . . ?
C8 O29 Ce1 143.4(13) . 4_556 ?
C14 O30 Ce2 126.0(11) . . ?
C14 O31 Ce1 141.8(12) . 5_657 ?
Ce1 O32 H32C 108.2 . . ?
Ce1 O32 H32A 112.7 . . ?
H32C O32 H32A 108.8 . . ?
Ce1 O33 H33B 113.6 . . ?
Ce1 O33 H33C 112.8 . . ?
H33B O33 H33C 110.7 . . ?
Ce1 O34 H34B 111.0 . . ?
Ce1 O34 H34C 111.2 . . ?
H34B O34 H34C 109.2 . . ?
Ce1 O35 H35B 111.2 . . ?
Ce1 O35 H35C 111.2 . . ?
H35B O35 H35C 109.4 . . ?
Ce2 O36 H36B 112.4 . . ?
Ce2 O36 H36C 113.9 . . ?
H36B O36 H36C 110.8 . . ?
Ce2 O37 H37B 112.2 . . ?
Ce2 O37 H37C 112.1 . . ?
H37B O37 H37C 110.1 . . ?
Ce2 O38 H38B 112.4 . . ?
Ce2 O38 H38C 112.4 . . ?
H38B O38 H38C 110.1 . . ?
Ce2 O39 H39B 110.8 . . ?
Ce2 O39 H39C 112.1 . . ?
H39B O39 H39C 109.4 . . ?
H40C O40 H40D 108.6 . . ?
O4 Si1 O4 173.4(17) 2_655 . ?
O4 Si1 O2 113.3(11) 2_655 2_655 ?
O4 Si1 O2 66.3(11) . 2_655 ?
O4 Si1 O2 66.3(11) 2_655 . ?
O4 Si1 O2 113.3(11) . . ?
O2 Si1 O2 172.7(16) 2_655 . ?
O4 Si1 O3 111.2(12) 2_655 . ?
O4 Si1 O3 74.5(11) . . ?
O2 Si1 O3 111.8(11) 2_655 . ?
O2 Si1 O3 74.5(11) . . ?
O4 Si1 O3 74.5(11) 2_655 2_655 ?
O4 Si1 O3 111.2(12) . 2_655 ?
O2 Si1 O3 74.5(11) 2_655 2_655 ?
O2 Si1 O3 111.8(11) . 2_655 ?
O3 Si1 O3 70.8(16) . 2_655 ?
O4 Si1 O1 67.5(11) 2_655 . ?
O4 Si1 O1 106.9(11) . . ?
O2 Si1 O1 67.1(11) 2_655 . ?
O2 Si1 O1 106.8(11) . . ?
O3 Si1 O1 177.3(11) . . ?
O3 Si1 O1 106.4(11) 2_655 . ?
O4 Si1 O1 106.9(11) 2_655 2_655 ?
O4 Si1 O1 67.5(11) . 2_655 ?
O2 Si1 O1 106.8(11) 2_655 2_655 ?
O2 Si1 O1 67.1(11) . 2_655 ?
O3 Si1 O1 106.4(11) . 2_655 ?
O3 Si1 O1 177.3(11) 2_655 2_655 ?
O1 Si1 O1 76.3(15) . 2_655 ?
O25 C1 O24 125.7(17) . . ?
O25 C1 C2 115.7(15) . . ?
O24 C1 C2 118.5(15) . . ?
C3 C2 N1 120.7(17) . . ?
C3 C2 C1 126.0(16) . . ?
N1 C2 C1 113.2(15) . . ?
C2 C3 C4 120.5(19) . . ?
C2 C3 H3 119.8 . . ?
C4 C3 H3 119.8 . . ?
C3 C4 C5 118(2) . . ?
C3 C4 H4 120.9 . . ?
C5 C4 H4 120.9 . . ?
C4 C5 C6 118.9(19) . . ?
C4 C5 H5 120.5 . . ?
C6 C5 H5 120.5 . . ?
N1 C6 C5 122.2(17) . . ?
N1 C6 C7 114.8(18) . . ?
C5 C6 C7 122.8(18) . . ?
O27 C7 O26 124.2(17) . . ?
O27 C7 C6 119.4(19) . . ?
O26 C7 C6 116.2(17) . . ?
O29 C8 O28 125.5(18) . . ?
O29 C8 C9 120.5(17) . . ?
O28 C8 C9 114.0(16) . . ?
N2 C9 C10 123.4(18) . . ?
N2 C9 C8 115.8(17) . . ?
C10 C9 C8 120.8(17) . . ?
C9 C10 C11 117.2(19) . . ?
C9 C10 H10 121.4 . . ?
C11 C10 H10 121.4 . . ?
C12 C11 C10 118.9(19) . . ?
C12 C11 H11 120.6 . . ?
C10 C11 H11 120.6 . . ?
C13 C12 C11 119.8(19) . . ?
C13 C12 H12 120.1 . . ?
C11 C12 H12 120.1 . . ?
N2 C13 C12 122.7(17) . . ?
N2 C13 C14 113.8(16) . . ?
C12 C13 C14 123.4(18) . . ?
O30 C14 O31 124.7(18) . . ?
O30 C14 C13 117.8(16) . . ?
O31 C14 C13 117.5(17) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ce1 O31 2.470(13) 5_657 ?
Ce1 O26 2.485(12) . ?
Ce1 O24 2.503(13) . ?
Ce1 O35 2.510(13) . ?
Ce1 O29 2.562(13) 4_546 ?
Ce1 O32 2.579(14) . ?
Ce1 N1 2.601(14) . ?
Ce1 O34 2.643(14) . ?
Ce1 O33 2.658(14) . ?
Ce2 O25 2.445(12) . ?
Ce2 O27 2.481(13) 6_556 ?
Ce2 O37 2.487(13) . ?
Ce2 O30 2.521(12) . ?
Ce2 O36 2.544(13) . ?
Ce2 O28 2.552(12) . ?
Ce2 O38 2.572(12) . ?
Ce2 N2 2.607(15) . ?
Ce2 O39 2.638(11) . ?
Mo1 O17 1.64(2) . ?
Mo1 O6 1.861(19) 2_655 ?
Mo1 O6 1.861(19) . ?
Mo1 O5 1.96(2) . ?
Mo1 O5 1.96(2) 2_655 ?
Mo1 O1 2.47(2) 2_655 ?
Mo1 O1 2.47(2) . ?
Mo2 O18 1.65(2) . ?
Mo2 O15 1.839(16) 2_655 ?
Mo2 O5 1.85(2) . ?
Mo2 O13 1.873(17) . ?
Mo2 O7 1.890(16) . ?
Mo2 O1 2.33(2) . ?
Mo2 O4 2.39(2) 2_655 ?
Mo3 O19 1.664(15) . ?
Mo3 O13 1.857(17) 2_655 ?
Mo3 O8 1.871(15) . ?
Mo3 O9 1.907(15) . ?
Mo3 O6 1.925(19) . ?
Mo3 O1 2.35(2) 2_655 ?
Mo3 O2 2.36(2) . ?
Mo4 O20 1.641(13) . ?
Mo4 O14 1.876(16) . ?
Mo4 O10 1.888(15) . ?
Mo4 O7 1.908(15) . ?
Mo4 O8 1.922(14) . ?
Mo4 O2 2.35(2) . ?
Mo4 O4 2.38(2) 2_655 ?
Mo5 O21 1.629(14) . ?
Mo5 O16 1.856(15) 2_655 ?
Mo5 O9 1.909(15) . ?
Mo5 O10 1.910(14) . ?
Mo5 O11 1.925(18) . ?
Mo5 O3 2.36(2) . ?
Mo5 O2 2.48(2) . ?
Mo6 O22 1.668(13) . ?
Mo6 O14 1.856(16) 2_655 ?
Mo6 O11 1.915(16) . ?
Mo6 O12 1.95(2) . ?
Mo6 O15 1.968(17) . ?
Mo6 O3 2.36(2) . ?
Mo6 O4 2.47(2) . ?
Mo7 O23 1.70(2) 2_655 ?
Mo7 O23 1.70(2) . ?
Mo7 O12 1.81(2) 2_655 ?
Mo7 O12 1.81(2) . ?
Mo7 O16 1.884(16) 2_655 ?
Mo7 O16 1.884(16) . ?
Mo7 O3 2.40(2) 2_655 ?
Mo7 O3 2.40(2) . ?
N1 C6 1.32(2) . ?
N1 C2 1.37(2) . ?
N2 C9 1.35(2) . ?
N2 C13 1.36(2) . ?
O1 Si1 1.65(2) . ?
O1 O4 1.79(3) 2_655 ?
O1 O2 1.81(3) 2_655 ?
O1 Mo3 2.35(2) 2_655 ?
O2 Si1 1.61(2) . ?
O2 O4 1.74(3) 2_655 ?
O2 O1 1.81(3) 2_655 ?
O3 Si1 1.64(2) . ?
O4 Si1 1.57(2) . ?
O4 O2 1.74(3) 2_655 ?
O4 O1 1.79(3) 2_655 ?
O4 Mo4 2.38(2) 2_655 ?
O4 Mo2 2.39(2) 2_655 ?
O13 Mo3 1.857(17) 2_655 ?
O14 Mo6 1.856(16) 2_655 ?
O15 Mo2 1.839(16) 2_655 ?
O16 Mo5 1.856(15) 2_655 ?
O23 O23 0.95(5) 2_655 ?
O24 C1 1.27(2) . ?
O25 C1 1.26(2) . ?
O26 C7 1.27(2) . ?
O27 C7 1.24(2) . ?
O27 Ce2 2.481(12) 6 ?
O28 C8 1.27(2) . ?
O29 C8 1.24(2) . ?
O29 Ce1 2.562(13) 4_556 ?
O30 C14 1.25(2) . ?
O31 C14 1.26(2) . ?
O31 Ce1 2.470(13) 5_657 ?
O32 H32C 0.8500 . ?
O32 H32A 0.8500 . ?
O33 H33B 0.8499 . ?
O33 H33C 0.8500 . ?
O34 H34B 0.8501 . ?
O34 H34C 0.8500 . ?
O35 H35B 0.8500 . ?
O35 H35C 0.8500 . ?
O36 H36B 0.8501 . ?
O36 H36C 0.8500 . ?
O37 H37B 0.8500 . ?
O37 H37C 0.8500 . ?
O38 H38B 0.8499 . ?
O38 H38C 0.8500 . ?
O39 H39B 0.8500 . ?
O39 H39C 0.8500 . ?
O40 H40C 0.8500 . ?
O40 H40D 0.8499 . ?
Si1 O4 1.57(2) 2_655 ?
Si1 O2 1.61(2) 2_655 ?
Si1 O3 1.64(2) 2_655 ?
Si1 O1 1.65(2) 2_655 ?
C1 C2 1.50(2) . ?
C2 C3 1.36(2) . ?
C3 C4 1.38(3) . ?
C3 H3 0.9300 . ?
C4 C5 1.38(3) . ?
C4 H4 0.9300 . ?
C5 C6 1.39(3) . ?
C5 H5 0.9300 . ?
C6 C7 1.49(3) . ?
C8 C9 1.51(3) . ?
C9 C10 1.39(3) . ?
C10 C11 1.43(3) . ?
C10 H10 0.9300 . ?
C11 C12 1.39(3) . ?
C11 H11 0.9300 . ?
C12 C13 1.37(2) . ?
C12 H12 0.9300 . ?
C13 C14 1.48(2) . ?
